Your SlideShare is downloading.
×

×

Saving this for later?
Get the SlideShare app to save on your phone or tablet. Read anywhere, anytime – even offline.

Text the download link to your phone

Standard text messaging rates apply

Like this document? Why not share!

- [Solutions manual] engineering ma... by sametron90 90697 views
- Calister solution by Sudhanshu Nayak 21186 views
- CIVE2700 solution manual by gurkang 8078 views
- Materiales the science and engine... by Meylis Hydyrow 5407 views
- solution for Materials Science and ... by shayangreen 4598 views
- Callister 7ed by Leandro Fabris 3323 views
- Materials science and engineering by Mit 3779 views
- Materials science and engineering c... by kitcrocodile12321 791 views
- Materials science and engineering 8... by Nile Haynes-Irby 1077 views
- Fundamentals of materials_science_a... by University of Syi... 660 views
- Materials science and engineering a... by Muhammad Abdullah... 1103 views
- Callister fundamentals of materia... by p09ch807 671 views

Like this? Share it with your network
Share

No Downloads

Total Views

36,965

On Slideshare

0

From Embeds

0

Number of Embeds

0

Shares

0

Downloads

1,551

Comments

0

Likes

32

No embeds

No notes for slide

- 1. CHAPTER 2 ATOMIC STRUCTURE AND INTERATOMIC BONDING PROBLEM SOLUTIONS Fundamental Concepts Electrons in Atoms 2.1 Cite the difference between atomic mass and atomic weight. Solution Atomic mass is the mass of an individual atom, whereas atomic weight is the average (weighted) of theatomic masses of an atoms naturally occurring isotopes.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 2. 50 2.2 Chromium has four naturally-occurring isotopes: 4.34% of Cr, with an atomic weight of 49.9460 52 53amu, 83.79% of Cr, with an atomic weight of 51.9405 amu, 9.50% of Cr, with an atomic weight of 52.9407 amu,and 2.37% of 54Cr, with an atomic weight of 53.9389 amu. On the basis of these data, confirm that the averageatomic weight of Cr is 51.9963 amu. Solution The average atomic weight of silicon (ACr ) is computed by adding fraction-of-occurrence/atomic weightproducts for the three isotopes. Thus ACr = f 50 A + f 52 A + f 53 A + f 54 A Cr 50Cr Cr 52Cr Cr 53Cr Cr 54Cr= (0.0434)(49.9460 amu) + (0.8379)(51.9405 amu) + (0.0950)(52.9407 amu) + (0.0237)(53.9389 amu) = 51.9963 amuExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 3. 2.3 (a) How many grams are there in one amu of a material? (b) Mole, in the context of this book, is taken in units of gram-mole. On this basis, how many atomsare there in a pound-mole of a substance? Solution (a) In order to determine the number of grams in one amu of material, appropriate manipulation of theamu/atom, g/mol, and atom/mol relationships is all that is necessary, as 1 mol 1 g / mol # g/amu = 6.022 × 10 23 atoms 1 amu / atom = 1.66 × 10-24 g/amu (b) Since there are 453.6 g/lbm, 1 lb - mol = (453.6 g/lb m ) (6.022 × 10 23 atoms/g - mol) = 2.73 × 1026 atoms/lb-molExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 4. 2.4 (a) Cite two important quantum-mechanical concepts associated with the Bohr model of the atom. (b) Cite two important additional refinements that resulted from the wave-mechanical atomic model. Solution (a) Two important quantum-mechanical concepts associated with the Bohr model of the atom are (1) thatelectrons are particles moving in discrete orbitals, and (2) electron energy is quantized into shells. (b) Two important refinements resulting from the wave-mechanical atomic model are (1) that electronposition is described in terms of a probability distribution, and (2) electron energy is quantized into both shells andsubshells--each electron is characterized by four quantum numbers.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 5. 2.5 Relative to electrons and electron states, what does each of the four quantum numbers specify? Solution The n quantum number designates the electron shell. The l quantum number designates the electron subshell. The ml quantum number designates the number of electron states in each electron subshell. The ms quantum number designates the spin moment on each electron.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 6. 2.6 Allowed values for the quantum numbers of electrons are as follows: n = 1, 2, 3, . . . l = 0, 1, 2, 3, . . . , n –1 m l = 0, ±1, ±2, ±3, . . . , ±l 1 ms = ± 2The relationships between n and the shell designations are noted in Table 2.1. Relative to the subshells, l = 0 corresponds to an s subshell l = 1 corresponds to a p subshell l = 2 corresponds to a d subshell l = 3 corresponds to an f subshellFor the K shell, the four quantum numbers for each of the two electrons in the 1s state, in the order of nlm l m s , are 1 1100( ) and 100( − ). Write the four quantum numbers for all of the electrons in the L and M shells, and note 2 2which correspond to the s, p, and d subshells. Solution For the L state, n = 2, and eight electron states are possible. Possible l values are 0 and 1, while possible ml 1 1values are 0 and ±1; and possible ms values are ± . Therefore, for the s states, the quantum numbers are 200 ( ) 2 2 1 1 1 1 1 1and 200 (− ) . For the p states, the quantum numbers are 210 ( ) , 210 (− ) , 211 ( ) , 211 (− ) , 21(−1)( ) , and 2 2 2 2 2 2 121(−1)(− ) . 2 For the M state, n = 3, and 18 states are possible. Possible l values are 0, 1, and 2; possible ml values are 1 10, ±1, and ±2; and possible ms values are ± . Therefore, for the s states, the quantum numbers are 300 ( ) , 2 2 1 1 1 1 1 1 1300 (− ) , for the p states they are 310 ( ) , 310 (− ) , 311 ( ) , 311 (− ) , 31(−1)( ) , and 31 (−1)(− ) ; for the d 2 2 2 2 2 2 2 1 1 1 1 1 1 1 1 1states they are 320 ( ) , 320 (− ) , 321 ( ) , 321 (− ) , 32 (−1)( ) , 32 (−1) (− ) , 322 ( ) , 322 (− ) , 32 (−2)( ) , 2 2 2 2 2 2 2 2 2 1and 32 (−2) (− ) . 2Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 7. 2.7 Give the electron configurations for the following ions: Fe2+, Al3+, Cu+, Ba2+, Br-, and O2-. Solution The electron configurations for the ions are determined using Table 2.2 (and Figure 2.6). Fe2+: From Table 2.2, the electron configuration for an atom of iron is 1s22s22p63s23p63d64s2. In order tobecome an ion with a plus two charge, it must lose two electrons—in this case the two 4s. Thus, the electronconfiguration for an Fe2+ ion is 1s22s22p63s23p63d6. Al3+: From Table 2.2, the electron configuration for an atom of aluminum is 1s22s22p63s23p1. In order tobecome an ion with a plus three charge, it must lose three electrons—in this case two 3s and the one 3p. Thus, theelectron configuration for an Al3+ ion is 1s22s22p6. Cu+: From Table 2.2, the electron configuration for an atom of copper is 1s22s22p63s23p63d104s1. In orderto become an ion with a plus one charge, it must lose one electron—in this case the 4s. Thus, the electronconfiguration for a Cu+ ion is 1s22s22p63s23p63d10. Ba2+: The atomic number for barium is 56 (Figure 2.6), and inasmuch as it is not a transition element theelectron configuration for one of its atoms is 1s22s22p63s23p63d104s24p64d105s25p66s2. In order to become an ionwith a plus two charge, it must lose two electrons—in this case two the 6s. Thus, the electron configuration for aBa2+ ion is 1s22s22p63s23p63d104s24p64d105s25p6. Br-: From Table 2.2, the electron configuration for an atom of bromine is 1s22s22p63s23p63d104s24p5. Inorder to become an ion with a minus one charge, it must acquire one electron—in this case another 4p. Thus, theelectron configuration for a Br- ion is 1s22s22p63s23p63d104s24p6. O2-: From Table 2.2, the electron configuration for an atom of oxygen is 1s22s22p4. In order to become anion with a minus two charge, it must acquire two electrons—in this case another two 2p. Thus, the electronconfiguration for an O2- ion is 1s22s22p6.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 8. 2.8 Sodium chloride (NaCl) exhibits predominantly ionic bonding. The Na+ and Cl- ions have electronstructures that are identical to which two inert gases? Solution + The Na ion is just a sodium atom that has lost one electron; therefore, it has an electron configuration thesame as neon (Figure 2.6). - The Cl ion is a chlorine atom that has acquired one extra electron; therefore, it has an electronconfiguration the same as argon.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 9. The Periodic Table 2.9 With regard to electron configuration, what do all the elements in Group VIIA of the periodic tablehave in common? Solution Each of the elements in Group VIIA has five p electrons.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 10. 2.10 To what group in the periodic table would an element with atomic number 114 belong? Solution From the periodic table (Figure 2.6) the element having atomic number 114 would belong to group IVA.According to Figure 2.6, Ds, having an atomic number of 110 lies below Pt in the periodic table and in the right-most column of group VIII. Moving four columns to the right puts element 114 under Pb and in group IVA.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 11. 2.11 Without consulting Figure 2.6 or Table 2.2, determine whether each of the electron configurationsgiven below is an inert gas, a halogen, an alkali metal, an alkaline earth metal, or a transition metal. Justify yourchoices. (a) 1s22s22p63s23p63d74s2 (b) 1s22s22p63s23p6 (c) 1s22s22p5 (d) 1s22s22p63s2 (e) 1s22s22p63s23p63d24s2 (f) 1s22s22p63s23p64s1 Solution (a) The 1s22s22p63s23p63d74s2 electron configuration is that of a transition metal because of an incompleted subshell. (b) The 1s22s22p63s23p6 electron configuration is that of an inert gas because of filled 3s and 3p subshells. (c) The 1s22s22p5 electron configuration is that of a halogen because it is one electron deficient fromhaving a filled L shell. (d) The 1s22s22p63s2 electron configuration is that of an alkaline earth metal because of two s electrons. (e) The 1s22s22p63s23p63d24s2 electron configuration is that of a transition metal because of an incompleted subshell. (f) The 1s22s22p63s23p64s1 electron configuration is that of an alkali metal because of a single s electron.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 12. 2.12 (a) What electron subshell is being filled for the rare earth series of elements on the periodic table? (b) What electron subshell is being filled for the actinide series? Solution (a) The 4f subshell is being filled for the rare earth series of elements. (b) The 5f subshell is being filled for the actinide series of elements.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 13. Bonding Forces and Energies 2.13 Calculate the force of attraction between a K+ and an O2- ion the centers of which are separated by adistance of 1.5 nm. Solution The attractive force between two ions FA is just the derivative with respect to the interatomic separation ofthe attractive energy expression, Equation 2.8, which is just A d− dE A r A FA = = = dr dr r2The constant A in this expression is defined in footnote 3. Since the valences of the K+ and O2- ions (Z1 and Z2) are+1 and -2, respectively, Z1 = 1 and Z2 = 2, then (Z1e) (Z 2 e) FA = 4πε0r 2 (1)(2)(1.602 × 10−19 C) 2 = (4)(π) (8.85 × 10−12 F/m) (1.5 × 10−9 m) 2 = 2.05 × 10-10 NExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 14. 2.14 The net potential energy between two adjacent ions, E N , may be represented by the sum of Equations2.8 and 2.9; that is, A B EN = − + n r rCalculate the bonding energy E 0 in terms of the parameters A, B, and n using the following procedure: 1. Differentiate E N with respect to r, and then set the resulting expression equal to zero, since the curve ofE N versus r is a minimum at E 0 . 2. Solve for r in terms of A, B, and n, which yields r 0 , the equilibrium interionic spacing. 3. Determine the expression for E 0 by substitution of r 0 into Equation 2.11. Solution (a) Differentiation of Equation 2.11 yields A B d− d n dEN r r = + dr dr dr A nB = − = 0 r (1 + 1) r (n + 1) (b) Now, solving for r (= r0) A nB 2 = (n + 1) r0 r0or A 1/(1 - n) r0 = nB (c) Substitution for r0 into Equation 2.11 and solving for E (= E0) A B E0 = − + n r0 r0 A B = − + A 1/(1 - n) A n/(1 - n) nB nB Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 15. 2.15 For a K+–Cl– ion pair, attractive and repulsive energies EA and ER, respectively, depend on thedistance between the ions r, according to 1.436 EA = − r 5.8 × 10−6 ER = r9For these expressions, energies are expressed in electron volts per K+–Cl– pair, and r is the distance in nanometers.The net energy E N is just the sum of the two expressions above. (a) Superimpose on a single plot E N , E R , and E A versus r up to 1.0 nm. (b) On the basis of this plot, determine (i) the equilibrium spacing r 0 between the K+ and Cl– ions, and (ii)the magnitude of the bonding energy E 0 between the two ions. (c) Mathematically determine the r 0 and E 0 values using the solutions to Problem 2.14 and compare thesewith the graphical results from part (b). Solution(a) Curves of EA, ER, and EN are shown on the plot below. (b) From this plot r0 = 0.28 nm E0 = – 4.6 eVExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 16. (c) From Equation 2.11 for EN A = 1.436 B = 5.86 × 10-6 n=9Thus, A 1/(1 - n) r0 = nB 1.436 1/(1 - 9) = = 0.279 nm (8)(5.86 × 10 -6 ) and A B E0 = − + A 1/(1 - n) A n/(1 - n) nB nB 1.436 5.86 × 10−6 = − + 1/(1 − 9) 9 /(1 − 9) 1.436 1.436 (9)( 5.86 × 10−6 ) (9)( 5.86 × 10−6 ) = – 4.57 eVExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 17. 2.16 Consider a hypothetical X+-Y- ion pair for which the equilibrium interionic spacing and bondingenergy values are 0.35 nm and -6.13 eV, respectively. If it is known that n in Equation 2.11 has a value of 10, usingthe results of Problem 2.14, determine explicit expressions for attractive and repulsive energies E A and E R ofEquations 2.8 and 2.9. Solution This problem gives us, for a hypothetical X+-Y- ion pair, values for r0 (0.35 nm), E0 (– 6.13 eV), and n(10), and asks that we determine explicit expressions for attractive and repulsive energies of Equations 2.8 and 2.9.In essence, it is necessary to compute the values of A and B in these equations. Expressions for r0 and E0 in termsof n, A, and B were determined in Problem 2.14, which are as follows: A 1/(1 - n) r0 = nB A B E0 = − + A 1/(1 - n) A n/(1 - n) nB nB Thus, we have two simultaneous equations with two unknowns (viz. A and B). Upon substitution of values for r0and E0 in terms of n, these equations take the forms A 1/(1 - 10) A -1/9 0.35 nm = = 10 B 10 B and A B − 6.13 eV = − 1/(1 − 10) + 10 /(1 − 10) A A 10 B 10 B A B = − −1/ 9 + A A −10 / 9 10B 10B We now want to solve these two equations simultaneously for values of A and B. From the first of these twoequations, solving for A/8B leads toExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 18. A = (0.35 nm) -9 10BFurthermore, from the above equation the A is equal to A = 10B(0.35 nm) -9When the above two expressions for A/10B and A are substituted into the above expression for E0 (- 6.13 eV), thefollowing results A B −6.13 eV = = − −1/ 9 + A A −10 / 9 10B 10B 10B(0.35 nm) -9 B = − −1/ 9 + −10 / 9 [(0.35 nm) -9] [(0.35 nm) -9 ] 10B(0.35 nm) -9 B = − + 0.35 nm (0.35 nm)10Or 10B B 9B −6.13 eV = = − 10 + 10 = − (0.35 nm) (0.35 nm) (0.35 nm)10Solving for B from this equation yields B = 1.88 × 10 -5 eV - nm10Furthermore, the value of A is determined from one of the previous equations, as follows: A = 10B(0.35 nm) -9 = (10)(1.88 × 10 -5 eV - nm10 )(0.35 nm) -9 = 2.39 eV - nmThus, Equations 2.8 and 2.9 becomeExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 19. 2.39 EA = − r 1.88 × 10−5 ER = r 10Of course these expressions are valid for r and E in units of nanometers and electron volts, respectively.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 20. 2.17 The net potential energy E N between two adjacent ions is sometimes represented by the expression C r EN = − + DÊxp− e (2.12) r ρin which r is the interionic separation and C, D, and ρ are constants whose values depend on the specific material. (a) Derive an expression for the bonding energy E 0 in terms of the equilibrium interionic separation r 0 andthe constants D and ρ using the following procedure: 1. Differentiate E N with respect to r and set the resulting expression equal to zero. 2. Solve for C in terms of D, ρ, and r 0 . 3. Determine the expression for E 0 by substitution for C in Equation 2.12. (b) Derive another expression for E 0 in terms of r 0 , C, and ρ using a procedure analogous to the oneoutlined in part (a). Solution (a) Differentiating Equation 2.12 with respect to r yields C r d− dD exp− dE r ρ = − dr dr dr C De− r /ρ = − r2 ρAt r = r0, dE/dr = 0, and C De−(r0 /ρ) = (2.12b) r02 ρSolving for C and substitution into Equation 2.12 yields an expression for E0 as r E0 = De−(r0 /ρ) 1 − 0 ρ (b) Now solving for D from Equation 2.12b above yields Cρ e (r0 /ρ) D = r02Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 21. Substitution of this expression for D into Equation 2.12 yields an expression for E0 as C ρ E0 = − 1 r0 r0 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 22. Primary Interatomic Bonds 2.18 (a) Briefly cite the main differences between ionic, covalent, and metallic bonding. (b) State the Pauli exclusion principle. Solution (a) The main differences between the various forms of primary bonding are: Ionic--there is electrostatic attraction between oppositely charged ions. Covalent--there is electron sharing between two adjacent atoms such that each atom assumes astable electron configuration. Metallic--the positively charged ion cores are shielded from one another, and also "glued"together by the sea of valence electrons. (b) The Pauli exclusion principle states that each electron state can hold no more than two electrons, whichmust have opposite spins.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 23. 2.19 Compute the percents ionic character of the interatomic bonds for the following compounds: TiO 2 ,ZnTe, CsCl, InSb, and MgCl 2 . Solution The percent ionic character is a function of the electron negativities of the ions XA and XB according toEquation 2.10. The electronegativities of the elements are found in Figure 2.7. For TiO2, XTi = 1.5 and XO = 3.5, and therefore, 2 %IC = 1 − e(− 0.25)(3.5−1.5) × 100 = 63.2% For ZnTe, XZn = 1.6 and XTe = 2.1, and therefore, 2 %IC = 1 − e (− 0.25) (2.1−1.6) × 100 = 6.1% For CsCl, XCs = 0.7 and XCl = 3.0, and therefore, 2 %IC = 1 − e(− 0.25)(3.0− 0.7) × 100 = 73.4% For InSb, XIn = 1.7 and XSb = 1.9, and therefore, 2 %IC = 1 − e(− 0.25)(1.9−1.7) × 100 = 1.0% For MgCl2, XMg = 1.2 and XCl = 3.0, and therefore, 2 %IC = 1 − e(− 0.25)(3.0−1.2) × 100 = 55.5% Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 24. 2.20 Make a plot of bonding energy versus melting temperature for the metals listed in Table 2.3. Usingthis plot, approximate the bonding energy for copper, which has a melting temperature of 1084°C. Solution Below is plotted the bonding energy versus melting temperature for these four metals. From this plot, thebonding energy for copper (melting temperature of 1084°C) should be approximately 3.6 eV. The experimentalvalue is 3.5 eV.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 25. 2.21 Using Table 2.2, determine the number of covalent bonds that are possible for atoms of the followingelements: germanium, phosphorus, selenium, and chlorine. Solution For germanium, having the valence electron structure 4s24p2, N = 4; thus, there are 8 – N = 4 covalentbonds per atom. For phosphorus, having the valence electron structure 3s23p3, N = 5; thus, there is 8 – N = 3 covalentbonds per atom. For selenium, having the valence electron structure 4s24p4, N = 6; thus, there are 8 – N = 2 covalentbonds per atom. For chlorine, having the valence electron structure 3s23p5, N = 7; thus, there are 8 – N = 1 covalent bondper atom.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 26. 2.22 What type(s) of bonding would be expected for each of the following materials: brass (a copper-zincalloy), rubber, barium sulfide (BaS), solid xenon, bronze, nylon, and aluminum phosphide (AlP)? Solution For brass, the bonding is metallic since it is a metal alloy. For rubber, the bonding is covalent with some van der Waals. (Rubber is composed primarily of carbonand hydrogen atoms.) For BaS, the bonding is predominantly ionic (but with some covalent character) on the basis of the relativepositions of Ba and S in the periodic table. For solid xenon, the bonding is van der Waals since xenon is an inert gas. For bronze, the bonding is metallic since it is a metal alloy (composed of copper and tin). For nylon, the bonding is covalent with perhaps some van der Waals. (Nylon is composed primarily ofcarbon and hydrogen.) For AlP the bonding is predominantly covalent (but with some ionic character) on the basis of the relativepositions of Al and P in the periodic table.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 27. Secondary Bonding or van der Waals Bonding 2.23 Explain why hydrogen fluoride (HF) has a higher boiling temperature than hydrogen chloride (HCl)(19.4 vs. –85°C), even though HF has a lower molecular weight. Solution The intermolecular bonding for HF is hydrogen, whereas for HCl, the intermolecular bonding is van derWaals. Since the hydrogen bond is stronger than van der Waals, HF will have a higher melting temperature.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 28. CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Solution Atomic structure relates to the number of protons and neutrons in the nucleus of an atom, as well as thenumber and probability distributions of the constituent electrons. On the other hand, crystal structure pertains to thearrangement of atoms in the crystalline solid material.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 29. Unit Cells Metallic Crystal Structures 3.2 If the atomic radius of aluminum is 0.143 nm, calculate the volume of its unit cell in cubic meters. Solution For this problem, we are asked to calculate the volume of a unit cell of aluminum. Aluminum has an FCCcrystal structure (Table 3.1). The FCC unit cell volume may be computed from Equation 3.4 as VC = 16R 3 2 = (16) (0.143 × 10 -9 m) 3( 2 ) = 6.62 × 10 -29 m3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 30. 3.3 Show for the body-centered cubic crystal structure that the unit cell edge length a and the atomicradius R are related through a =4R/ 3 . Solution Consider the BCC unit cell shown belowUsing the triangle NOP (NP) 2 = a 2 + a 2 = 2a 2And then for triangle NPQ, (NQ) 2 = (QP) 2 + ( NP) 2But NQ = 4R, R being the atomic radius. Also, QP = a. Therefore, (4R) 2 = a 2 + 2a 2or 4R a = 3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 31. 3.4 For the HCP crystal structure, show that the ideal c/a ratio is 1.633. Solution A sketch of one-third of an HCP unit cell is shown below.Consider the tetrahedron labeled as JKLM, which is reconstructed asThe atom at point M is midway between the top and bottom faces of the unit cell--that is MH = c/2. And, sinceatoms at points J, K, and M, all touch one another, JM = JK = 2R = awhere R is the atomic radius. Furthermore, from triangle JHM, (JM ) 2 = ( JH ) 2 + ( MH ) 2orExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 32. c 2 a 2 = (JH ) 2 + 2 Now, we can determine the JH length by consideration of triangle JKL, which is an equilateral triangle, a /2 3 cos 30° = = JH 2and a JH = 3Substituting this value for JH in the above expression yields a 2 c 2 a2 c2 a2 = + = + 3 2 3 4and, solving for c/a c 8 = = 1.633 a 3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 33. 3.5 Show that the atomic packing factor for BCC is 0.68. Solution The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or VS APF = VCSince there are two spheres associated with each unit cell for BCC 4πR 3 8πR 3 VS = 2(sphere volume) = 2 3 = 3Also, the unit cell has cubic symmetry, that is VC = a3. But a depends on R according to Equation 3.3, and 4R 3 64 R 3 VC = = 3 3 3Thus, VS 8π R 3 /3 APF = = = 0.68 VC 64 R 3 /3 3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 34. 3.6 Show that the atomic packing factor for HCP is 0.74. Solution The APF is just the total sphere volume-unit cell volume ratio. For HCP, there are the equivalent of sixspheres per unit cell, and thus 4π R 3 VS = 6 3 = 8π R 3 Now, the unit cell volume is just the product of the base area times the cell height, c. This base area is just threetimes the area of the parallelepiped ACDE shown below.The area of ACDE is just the length of CD times the height BC . But CD is just a or 2R, and 2R 3 BC = 2R cos (30°) = 2Thus, the base area is just 2 R 3 2 AREA = (3)(CD)(BC) = (3)(2 R) = 6R 3 2 and since c = 1.633a = 2R(1.633) VC = (AREA)(c) = 6 R 2 c 3 (3.S1)Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 35. = (6 R 2 3 ) (2)(1.633)R = 12 3 (1.633) R 3Thus, VS 8π R 3 APF = = = 0.74 VC 12 3 (1.633) R 3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 36. Density Computations 3.7 Iron has a BCC crystal structure, an atomic radius of 0.124 nm, and an atomic weight of 55.85 g/mol.Compute and compare its theoretical density with the experimental value found inside the front cover. Solution This problem calls for a computation of the density of iron. According to Equation 3.5 nAFe ρ = VC N AFor BCC, n = 2 atoms/unit cell, and 4 R 3 VC = 3Thus, nAFe ρ = 4 R 3 NA 3 (2 atoms/unit cell)(55.85 g/mol) = [(4) (0.124 × 10-7 cm) / 3] /(unit cell) (6.022 × 1023 atoms/mol) 3 = 7.90 g/cm3The value given inside the front cover is 7.87 g/cm3.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 37. 3.8 Calculate the radius of an iridium atom, given that Ir has an FCC crystal structure, a density of 22.4 3g/cm , and an atomic weight of 192.2 g/mol. Solution We are asked to determine the radius of an iridium atom, given that Ir has an FCC crystal structure. ForFCC, n = 4 atoms/unit cell, and VC = 16R 3 2 (Equation 3.4). Now, nAIr ρ = VC N A nAIr = (16R 3 2 ) N AAnd solving for R from the above expression yields nA 1/3 R = Ir 16 ρN A 2 (4 atoms/unit cell) (192.2 g/mol) 1/3 = (16)(22.4 g/cm 3)(6.022 × 10 23 atoms/mol )( 2 ) = 1.36 × 10-8 cm = 0.136 nmExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 38. 3.9 Calculate the radius of a vanadium atom, given that V has a BCC crystal structure, a density of 5.96 3g/cm , and an atomic weight of 50.9 g/mol. Solution This problem asks for us to calculate the radius of a vanadium atom. For BCC, n = 2 atoms/unit cell, and 4 R 3 64 R 3 VC = = 3 3 3Since, from Equation 3.5 nAV ρ = VC N A nAV = 64 R 3 N A 3 3 and solving for R the previous equation 3 3nA 1/3 R = V 64 ρ N A and incorporating values of parameters given in the problem statement 1/3 R= (3 3) (2 atoms/unit cell) (50.9 g/mol) (64) (5.96 g/cm3)(6.022 × 10 23 atoms/mol ) = 1.32 × 10-8 cm = 0.132 nmExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 39. 3.10 Some hypothetical metal has the simple cubic crystal structure shown in Figure 3.24. If its atomicweight is 70.4 g/mol and the atomic radius is 0.126 nm, compute its density. Solution For the simple cubic crystal structure, the value of n in Equation 3.5 is unity since there is only a singleatom associated with each unit cell. Furthermore, for the unit cell edge length, a = 2R (Figure 3.24). Therefore,employment of Equation 3.5 yields nA nA ρ = = VC N A (2 R) 3 N Aand incorporating values of the other parameters provided in the problem statement leads to (1 atom/unit cell)(70.4 g/mol) ρ= -8 3 (2)(1.26 × 10 cm) /(unit cell) (6.022 × 10 23 atoms/mol ) 7.31 g/cm3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 40. 3.11 Zirconium has an HCP crystal structure and a density of 6.51 g/cm3. (a) What is the volume of its unit cell in cubic meters? (b) If the c/a ratio is 1.593, compute the values of c and a. Solution (a) The volume of the Zr unit cell may be computed using Equation 3.5 as nAZr VC = ρN ANow, for HCP, n = 6 atoms/unit cell, and for Zr, AZr = 91.22 g/mol. Thus, (6 atoms/unit cell)(91.22 g/mol) VC = (6.51 g/cm3)(6.022 × 10 23 atoms/mol ) = 1.396 × 10-22 cm3/unit cell = 1.396 × 10-28 m3/unit cell (b) From Equation 3.S1 of the solution to Problem 3.6, for HCP VC = 6 R 2 c 3But, since a = 2R, (i.e., R = a/2) then a 2 3 3 a2c VC = 6 c 3 = 2 2but, since c = 1.593a 3 3 (1.593) a 3 VC = = 1.396 × 10 -22 cm3/unit cell 2Now, solving for a (2)(1.396 × 10 -22 cm3 ) 1/3 a = (3) ( 3) (1.593) Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 41. = 3.23 × 10-8 cm = 0.323 nmAnd finally c = 1.593a = (1.593)(0.323 nm) = 0.515 nmExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 42. 3.12 Using atomic weight, crystal structure, and atomic radius data tabulated inside the front cover,compute the theoretical densities of lead, chromium, copper, and cobalt, and then compare these values with themeasured densities listed in this same table. The c/a ratio for cobalt is 1.623. Solution Since Pb has an FCC crystal structure, n = 4, and VC = 16R 3 2 (Equation 3.4). Also, R = 0.175 nm (1.75× 10-8 cm) and APb = 207.2 g/mol. Employment of Equation 3.5 yields nAPb ρ = VC N A (4 atoms/unit cell)(207.2 g/mol) = {(16)(1.75 × 10-8 cm)3( 2 )]/(unit cell) } 6.022 × 1023 atoms/mol) [ ( = 11.35 g/cm3The value given in the table inside the front cover is 11.35 g/cm3. 4 R 3 Chromium has a BCC crystal structure for which n = 2 and VC = a3 = 3 (Equation 3.3); also ACr = 52.00g/mol and R = 0.125 nm. Therefore, employment of Equation 3.5 leads to (2 atoms/unit cell)(52.00 g/mol) ρ = (4)(1.25 × 10 -8 cm) 3 /(unit cell) (6.022 × 10 23 atoms/mol ) 3 = 7.18 g/cm3The value given in the table is 7.19 g/cm3. Copper also has an FCC crystal structure and therefore (4 atoms/unit cell)(63.55 g/mol) ρ = [ ] 3 (2)(1.28 × 10 -8 cm)( 2 ) /(unit cell) (6.022 × 10 23 atoms/mol ) = 8.90 g/cm3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 43. The value given in the table is 8.90 g/cm3. Cobalt has an HCP crystal structure, and from the solution to Problem 3.6 (Equation 3.S1), VC = 6R 2c 3and, since c = 1.623a and a = 2R, c = (1.623)(2R); hence VC = 6R 2 (1.623)(2R) 3 = (19.48)( 3)R 3 = (19.48)( 3)(1.25 × 10−8 cm) 3 = 6.59 × 10−23 cm3/unit cellAlso, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is nACo ρ = VC N A (6 atoms/unit cell)(58.93 g/mol) = (6.59 × 10 -23 cm3/unit cell)(6.022 × 10 23 atoms/mol ) = 8.91 g/cm3The value given in the table is 8.9 g/cm3.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 44. 3.13 Rhodium has an atomic radius of 0.1345 nm and a density of 12.41 g/cm3. Determine whether it hasan FCC or BCC crystal structure. Solution In order to determine whether Rh has an FCC or a BCC crystal structure, we need to compute its densityfor each of the crystal structures. For FCC, n = 4, and a = 2 R 2 (Equation 3.1). Also, from Figure 2.6, its atomicweight is 102.91 g/mol. Thus, for FCC (employing Equation 3.5) nARh nARh ρ = = a3N A (2R 2 )3 N A (4 atoms/unit cell)(102.91 g/mol) = [ ] 3 (2)(1.345 × 10 -8 cm)( 2 ) /(unit cell) (6.022 × 10 23 atoms / mol) = 12.41 g/cm3which is the value provided in the problem statement. Therefore, Rh has the FCC crystal structure.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 45. 3.14 Below are listed the atomic weight, density, and atomic radius for three hypothetical alloys. Foreach determine whether its crystal structure is FCC, BCC, or simple cubic and then justify your determination. Asimple cubic unit cell is shown in Figure 3.24. Alloy Atomic Weight Density Atomic Radius (g/mol) (g/cm3) (nm) A 77.4 8.22 0.125 B 107.6 13.42 0.133 C 127.3 9.23 0.142 Solution For each of these three alloys we need, by trial and error, to calculate the density using Equation 3.5, andcompare it to the value cited in the problem. For SC, BCC, and FCC crystal structures, the respective values of n 4Rare 1, 2, and 4, whereas the expressions for a (since VC = a3) are 2R, 2 R 2 , and . 3 For alloy A, let us calculate ρ assuming a simple cubic crystal structure. nAA ρ = VC N A nAA = (2R)3 N A (1 atom/unit cell)(77.4 g/mol) = [ ] 3 (2)(1.25 × 10−8 ) /(unit cell) (6.022 × 10 23 atoms/mol ) = 8.22 g/cm3Therefore, its crystal structure is simple cubic. For alloy B, let us calculate ρ assuming an FCC crystal structure. nAB ρ = (2 R 2) 3 N AExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 46. (4 atoms/unit cell)(107.6 g/mol) = [( ) ] 3 2 2 (1.33 × 10 -8 cm) /(unit cell) (6.022 × 10 23 atoms/mol ) = 13.42 g/cm3Therefore, its crystal structure is FCC. For alloy C, let us calculate ρ assuming a simple cubic crystal structure. nAC = (2R)3 N A (1 atom/unit cell)(127.3 g/mol) = [ ] 3 (2)(1.42 × 10 -8 cm) /(unit cell) (6.022 × 10 23 atoms/mol ) = 9.23 g/cm3Therefore, its crystal structure is simple cubic.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 47. 3.15 The unit cell for tin has tetragonal symmetry, with a and b lattice parameters of 0.583 and 0.318 nm,respectively. If its density, atomic weight, and atomic radius are 7.30 g/cm3, 118.69 g/mol, and 0.151 nm,respectively, compute the atomic packing factor. Solution In order to determine the APF for Sn, we need to compute both the unit cell volume (VC) which is just thea2c product, as well as the total sphere volume (VS) which is just the product of the volume of a single sphere andthe number of spheres in the unit cell (n). The value of n may be calculated from Equation 3.5 as ρVC N A n = ASn (7.30 g/cm3)(5.83) 2 (3.18)(× 10 -24 cm3)(6.022 × 10 23 atoms / mol) = 118.69 g/mol = 4.00 atoms/unit cellTherefore 4 (4) π R 3 V 3 APF = S = 2 (c) VC (a) 4 (4) (π)(1.51 × 10 -8 cm) 3 3 = (5.83 × 10 × -8 cm) 2 (3.18 10 -8 cm) = 0.534Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 48. 3.16 Iodine has an orthorhombic unit cell for which the a, b, and c lattice parameters are 0.479, 0.725,and 0.978 nm, respectively. (a) If the atomic packing factor and atomic radius are 0.547 and 0.177 nm, respectively, determine thenumber of atoms in each unit cell. (b) The atomic weight of iodine is 126.91 g/mol; compute its theoretical density. Solution (a) For indium, and from the definition of the APF 4 n π R3 V 3 APF = S = VC abcwe may solve for the number of atoms per unit cell, n, as (APF) abc n = 4 π R3 3Incorporating values of the above parameters provided in the problem state leads to (0.547)(4.79 × 10 -8 cm)(7.25 × 10 -8 cm) (9.78 × 10 -8 cm) = 4 π (1.77 × 10 -8 cm) 3 3 = 8.0 atoms/unit cell (b) In order to compute the density, we just employ Equation 3.5 as nAI ρ = abc N A (8 atoms/unit cell)(126.91 g/mol) = {(4.79 × [ 10 -8 ] } cm)(7.25 × 10 -8 cm) (9.78 × 10 -8 cm) / unit cell (6.022 × 10 23 atoms/mol ) = 4.96 g/cm3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 49. 3. 17 Titanium has an HCP unit cell for which the ratio of the lattice parameters c/a is 1.58. If the radiusof the Ti atom is 0.1445 nm, (a) determine the unit cell volume, and (b) calculate the density of Ti and compare itwith the literature value. Solution (a) We are asked to calculate the unit cell volume for Ti. For HCP, from Equation 3.S1 (found in thesolution to Problem 3.6) VC = 6 R 2 c 3But for Ti, c = 1.58a, and a = 2R, or c = 3.16R, and VC = (6)(3.16) R 3 3 [ ] 3 = (6) (3.16) ( 3) 1.445 × 10 -8 cm = 9.91 × 10−23 cm3/unit cell (b) The theoretical density of Ti is determined, using Equation 3.5, as follows: nATi ρ = VC N AFor HCP, n = 6 atoms/unit cell, and for Ti, ATi = 47.87 g/mol (as noted inside the front cover). Thus, (6 atoms/unit cell)(47.87 g/mol) ρ = (9.91 × 10 -23 cm3/unit cell)(6.022 × 10 23 atoms/mol ) = 4.81 g/cm3The value given in the literature is 4.51 g/cm3.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 50. 3.18 Zinc has an HCP crystal structure, a c/a ratio of 1.856, and a density of 7.13 g/cm3. Compute theatomic radius for Zn. Solution In order to calculate the atomic radius for Zn, we must use Equation 3.5, as well as the expression whichrelates the atomic radius to the unit cell volume for HCP; Equation 3.S1 (from Problem 3.6) is as follows: VC = 6 R 2 c 3In this case c = 1.856a, but, for HCP, a = 2R, which means that VC = 6 R 2 (1.856)(2R) 3 = (1.856)(12 3)R 3And from Equation 3.5, the density is equal to nAZn nAZn ρ = = VC N A (1.856)(12 3) R 3 N AAnd, solving for R from the above equation leads to the following: nAZn 1/3 R = (1.856) (12 3) ρ N A And incorporating appropriate values for the parameters in this equation leads to (6 atoms/unit cell) (65.41 g/mol) 1/3 R= (1.856) (12 3)(7.13 g/cm )(6.022 × 10 atoms/mol ) 3 23 = 1.33 × 10-8 cm = 0.133 nmExcerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 51. 3.19 Rhenium has an HCP crystal structure, an atomic radius of 0.137 nm, and a c/a ratio of 1.615.Compute the volume of the unit cell for Re. SolutionIn order to compute the volume of the unit cell for Re, it is necessary to use Equation 3.S1 (found in Problem 3.6),that is VC = 6 R 2 c 3The problem states that c = 1.615a, and a = 2R. Therefore VC = (1.615) (12 3) R 3 = (1.615) (12 3)(1.37 × 10 -8 cm) 3 = 8.63 × 10 -23 cm3 = 8.63 × 10 -2 nm3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 52. Crystal Systems 3.20 Below is a unit cell for a hypothetical metal. (a) To which crystal system does this unit cell belong? (b) What would this crystal structure be called? (c) Calculate the density of the material, given that its atomic weight is 141 g/mol. Solution (a) The unit cell shown in the problem statement belongs to the tetragonal crystal system since a = b =0.30 nm, c = 0.40 nm, and α = β = γ = 90°. (b) The crystal structure would be called body-centered tetragonal. (c) As with BCC, n = 2 atoms/unit cell. Also, for this unit cell VC = (3.0 × 10−8 cm) 2 ( 4.0 × 10−8 cm) = 3.60 × 10−23 cm3/unit cellThus, using Equation 3.5, the density is equal to nA ρ = VC N A (2 atoms/unit cell) (141 g/mol) = (3.60 × 10 -23 cm3/unit cell)(6.022 × 10 23 atoms/mol ) = 13.0 g/cm3Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 53. 3.21 Sketch a unit cell for the body-centered orthorhombic crystal structure. SolutionA unit cell for the body-centered orthorhombic crystal structure is presented below.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 54. Point Coordinates 3.22 List the point coordinates for all atoms that are associated with the FCC unit cell (Figure 3.1). Solution From Figure 3.1b, the atom located of the origin of the unit cell has the coordinates 000. Coordinates for 11other atoms in the bottom face are 100, 110, 010, and 0 . (The z coordinate for all these points is zero.) 22 11 For the top unit cell face, the coordinates are 001, 101, 111, 011, and 1. 22 Coordinates for those atoms that are positioned at the centers of both side faces, and centers of both front 11 11and back faces need to be specified. For the front and back-center face atoms, the coordinates are 1 and 0 , 22 22 1 1 1 1respectively. While for the left and right side center-face atoms, the respective coordinates are 0 and 1 . 2 2 2 2Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 55. 3.23 List the point coordinates of the titanium, barium, and oxygen ions for a unit cell of the perovskitecrystal structure (Figure 12.6). Solution In Figure 12.6, the barium ions are situated at all corner positions. The point coordinates for these ions areas follows: 000, 100, 110, 010, 001, 101, 111, and 011. 11 11 The oxygen ions are located at all face-centered positions; therefore, their coordinates are 0, 1, 22 22 11 11 1 1 1 11 , 0 , 0 , and 1 . 22 22 2 2 2 2 111 And, finally, the titanium ion resides at the center of the cubic unit cell, with coordinates . 222Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 56. 3.24 List the point coordinates of all atoms that are associated with the diamond cubic unit cell (Figure12.15). Solution First of all, one set of carbon atoms occupy all corner positions of the cubic unit cell; the coordinates ofthese atoms are as follows: 000, 100, 110, 010, 001, 101, 111, and 011. 11 Another set of atoms reside on all of the face-centered positions, with the following coordinates: 0, 2211 11 11 1 1 1 1 1, 1 , 0 , 0 , and 1 .22 22 22 2 2 2 2 The third set of carbon atoms are positioned within the interior of the unit cell. Using an x-y-z coordinatesystem oriented as in Figure 3.4, the coordinates of the atom that lies toward the lower-left-front of the unit cell has 311the coordinates , whereas the atom situated toward the lower-right-back of the unit cell has coordinates of 4441 31 11 3 . Also, the carbon atom that resides toward the upper-left-back of the unit cell has the coordinates.444 444 333And, the coordinates of the final atom, located toward the upper-right-front of the unit cell, are . 444Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 57. 1 1 1 1 3 3.25 Sketch a tetragonal unit cell , and within that cell indicate locations of the 1 and point 2 2 4 2 4coordinates. Solution 1 1 1 1 3A tetragonal unit in which are shown the 1 and point coordinates is presented below. 2 2 4 24Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 58. 3.26 Using the Molecule Definition Utility found in both “Metallic Crystal Structures andCrystallography” and “Ceramic Crystal Structures” modules of VMSE, located on the book’s web site[www.wiley.com/college/Callister (Student Companion Site)], generate a three-dimensional unit cell for theintermetallic compound AuCu 3 given the following: (1) the unit cell is cubic with an edge length of 0.374 nm, (2)gold atoms are situated at all cube corners, and (3) copper atoms are positioned at the centers of all unit cell faces. Solution First of all, open the “Molecular Definition Utility”; it may be found in either of “Metallic CrystalStructures and Crystallography” or “Ceramic Crystal Structures” modules. In the “Step 1” window, it is necessary to define the atom types, colors for the spheres (atoms), and specifyatom sizes. Let us enter “Au” as the name for the gold atoms (since “Au” the symbol for gold), and “Cu” as thename for the copper atoms. Next it is necessary to choose a color for each atom type from the selections that appearin the pull-down menu—for example, “Yellow” for Au and “Red” for Cu. In the “Atom Size” window, it isnecessary to enter an atom/ion size. In the instructions for this step, it is suggested that the atom/ion diameter innanometers be used. From the table found inside the front cover of the textbook, the atomic radii for gold andcopper are 0.144 nm and 0.128 nm, respectively, and, therefore, their ionic diameters are twice these values (i.e.,0.288 nm and 0.256 nm); therefore, we enter the values “0.288” and “0.256” for the two atom types. Now click onthe “Register” button, followed by clicking on the “Go to Step 2” button. In the “Step 2” window we specify positions for all of the atoms within the unit cell; their pointcoordinates are specified in the problem statement. Let’s begin with gold. Click on the yellow sphere that islocated to the right of the “Molecule Definition Utility” box. Again, Au atoms are situated at all eight corners of thecubic unit cell. One Au will be positioned at the origin of the coordinate system—i.e., its point coordinates are 000,and, therefore, we enter a “0” (zero) in each of the “x”, “y”, and “z” atom position boxes. Next we click on the“Register Atom Position” button. Now we enter the coordinates of another gold atom; let us arbitrarily select theone that resides at the corner of the unit cell that is one unit-cell length along the x-axis (i.e., at the 100 pointcoordinate). Inasmuch as it is located a distance of a units along the x-axis the value of “0.374” is entered in the “x”atom position box (since this is the value of a given in the problem statement); zeros are entered in each of the “y”and “z” position boxes. We repeat this procedure for the remaining six Au atoms. After this step has been completed, it is necessary to specify positions for the copper atoms, which arelocated at all six face-centered sites. To begin, we click on the red sphere that is located next to the “MoleculeDefinition Utility” box. The point coordinates for some of the Cu atoms are fractional ones; in these instances, the a 1 1unit cell length (i.e., 0.374) is multiplied by the fraction. For example, one Cu atom is located 1 coordinate. 2 2 1 1Therefore, the x, y, and z atoms positions are (1)(0.374) = 0.374, (0.374) = 0.187, and (0.374) = 0.187, 2 2respectively. For the gold atoms, the x, y, and z atom position entries for all 8 sets of point coordinates are as follows:Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 59. 0, 0, and 0 0.374, 0, and 0 0, 0.374, and 0 0, 0, and 0.374 0, 0.374, 0.374 0.374, 0, 0.374 0.374, 0.374, 0 0.374, 0.374, 0.374 Now, for the copper atoms, the x, y, and z atom position entries for all 6 sets of point coordinates are asfollows: 0.187, 0.187, 0 0.187, 0, 0.187 0, 0.187, 0.187 0.374, 0.187, 0.187 0.187, 0.374, 0.187 0.187, 0.187, 0.374 In Step 3, we may specify which atoms are to be represented as being bonded to one another, and whichtype of bond(s) to use (single solid, single dashed, double, and triple are possibilities), or we may elect to notrepresent any bonds at all (in which case we are finished). If it is decided to show bonds, probably the best thing todo is to represent unit cell edges as bonds. This image may be rotated by using mouse click-and-drag Your image should appear as the following screen shot. Here the gold atoms appear lighter than the copperatoms.Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 60. [Note: Unfortunately, with this version of the Molecular Definition Utility, it is not possible to save either the dataor the image that you have generated. You may use screen capture (or screen shot) software to record and storeyour image.]Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only tostudents enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permittedby Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.
- 61.

Be the first to comment